page_title: Heat treating
section_title: Effects of time and temperature
hierarchical_section_title: Heat treating / Effects of time and temperature
caption_attribution_description: Français&#160;: Diagramme temps, température, taux de transformation
context_page_description: Heat treating is a group of industrial, thermal and metalworking processes used to alter the physical, and sometimes chemical, properties of a material. The most common application is metallurgical. Heat treatments are also used in the manufacture of many other materials, such as glass. Heat treatment involves the use of heating or chilling, normally to extreme temperatures, to achieve the desired result such as hardening or softening of a material. Heat treatment techniques include annealing, case hardening, precipitation strengthening, tempering, carburizing, normalizing and quenching. Although the term heat treatment applies only to processes where the heating and cooling are done for the specific purpose of altering properties intentionally, heating and cooling often occur incidentally during other manufacturing processes such as hot forming or welding.
context_section_description: Proper heat treating requires precise control over temperature, time held at a certain temperature and cooling rate.
  With the exception of stress-relieving, tempering, and aging, most heat treatments begin by heating an alloy beyond a certain transformation, or arrest (A), temperature. This temperature is referred to as an "arrest" because at the A temperature the metal experiences a period of hysteresis. At this point, all of the heat energy is used to cause the crystal change, so the temperature stops rising for a short time (arrests) and then continues climbing once the change is complete. Therefore, the alloy must be heated above the critical temperature for a transformation to occur. The alloy will usually be held at this temperature long enough for the heat to completely penetrate the alloy, thereby bringing it into a complete solid solution. Iron, for example, has four critical-temperatures, depending on carbon content. Pure iron in its alpha (room temperature) state changes to nonmagnetic gamma-iron at its A₂ temperature, and weldable delta-iron at its A₄ temperature. However, as carbon is added, becoming steel, the A₂ temperature splits into the A₃ temperature, also called the austenizing temperature (all phases become austenite, a solution of gamma iron and carbon) and its A₁ temperature (austenite changes into pearlite upon cooling). Between these upper and lower temperatures the proeutectoid phase forms upon cooling.
  Because a smaller grain size usually enhances mechanical properties, such as toughness, shear strength and tensile strength, these metals are often heated to a temperature that is just above the upper critical-temperature, in order to prevent the grains of solution from growing too large. For instance, when steel is heated above the upper critical-temperature, small grains of austenite form. These grow larger as temperature is increased. When cooled very quickly, during a martensite transformation, the austenite grain-size directly affects the martensitic grain-size. Larger grains have large grain-boundaries, which serve as weak spots in the structure. The grain size is usually controlled to reduce the probability of breakage.
  The diffusion transformation is very time-dependent. Cooling a metal will usually suppress the precipitation to a much lower temperature. Austenite, for example, usually only exists above the upper critical temperature. However, if the austenite is cooled quickly enough, the transformation may be suppressed for hundreds of degrees below the lower critical temperature. Such austenite is highly unstable and, if given enough time, will precipitate into various microstructures of ferrite and cementite. The cooling rate can be used to control the rate of grain growth or can even be used to produce partially martensitic microstructures. However, the martensite transformation is time-independent. If the alloy is cooled to the martensite transformation (Mₛ) temperature before other microstructures can fully form, the transformation will usually occur at just under the speed of sound.
  When austenite is cooled slow enough that a martensite transformation does not occur, the austenite grain size will have an effect on the rate of nucleation, but it is generally temperature and the rate of cooling that controls the grain size and microstructure. When austenite is cooled extremely slow, it will form large ferrite crystals filled with spherical inclusions of cementite. This microstructure is referred to as "sphereoidite." If cooled a little faster, then coarse pearlite will form. Even faster, and fine pearlite will form. If cooled even faster, bainite will form. Similarly, these microstructures will also form if cooled to a specific temperature and then held there for a certain time.
  Most non-ferrous alloys are also heated in order to form a solution. Most often, these are then cooled very quickly to produce a martensite transformation, putting the solution into a supersaturated state. The alloy, being in a much softer state, may then be cold worked. This causes work hardening that incre
caption: Time-temperature transformation (TTT) diagram for steel. The red curves represent different cooling rates (velocity) when cooled from the upper critical (A3) temperature. V1 produces martensite. V2 has pearlite mixed with martensite, V3 produces bainite, along with pearlite and matensite.